Production Methods of Carbon Nanomaterials.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Different types of carbon nanotubes, carbon nanofibers, vapor grown carbon fiber and other types of carbon nanostructure materials can be produced in various ways. In this section, different techniques for nanotube, nanofibers synthesis and their status are in brief described. The most common techniques used nowadays are: arc discharge, laser ablation, chemical vapour deposition. Economically feasible large-scale production and purification techniques still have to be developed.
In the arc discharge, a vapor is created by an arc discharge between two carbon electrodes with or without catalyst. In the laser ablation technology a high achievement laser beam, impose to a volume of the carbon, containing feedstock gas (methane or carbon monoxide). Now laser ablation produces a very small amount of pure nanotubes, while an arc-discharge method produces in general large amounts of the impure material. CVD seems to be the most promising method for possible industrial scale-up due to the relatively low growth temperature, high yields and high purities that can be achieved.
This method creates nanotubes through arc-vaporisation of two carbon rods placed end to end, separated by approximately 1mm, in an enclosure that is usually filled with inert gas (helium, argon) at low pressure (between 50 and 700 mbar). Recent investigations have shown that it is also possible to create nanotubes with the arc method in liquid nitrogen. A direct current of 50 to 100 A driven by approximately 20 V creates a high temperature discharge between the two electrodes 2000-3000 °C. The discharge vaporises one of the carbon rods and forms a small rod shaped deposit on the other rod. Producing nanotubes in high yield depends on the uniformity of the plasma arc and the temperature of the deposit form on the carbon electrode
The Nanotubes created using this method are usually short tubes with diameters ranging from 0.6 to 1.4 nm for single walled and 10 nm diameter multi-walled nanotubes. These tubes can be single walled tubes or multiple walled nanotubes. This method is relatively easy to implement, and will produce yields of 30%. The nanotubes produced contain more impurities compared to other methods, and the consistency of the shape, wall, and lengths of the tubes are somewhat random [www.iljinnanotech.co.kr, 2002 and Journet and Bernier, 1998].
Figure 2.10 shows a schematic diagram of arc-discharge apparatus for the synthesis of carbon nanotubes. This apparatus must be connected both to a vacuum line with a diffusion pump, and to a helium supply. The electrodes are two graphite rods, usually of high purity. Typically, the anode is a long rod approximately 6 mm in diameter and the cathode a much shorter rod 9 mm in diameter. Efficient cooling of the cathode has been shown to be essential in producing good quality nanotubes [Iijima 1991; Ebbesen and Ajayan 1992; Ching-Hwa et al., 1995; Journet and Bernier, 1998; Jung et al., 2003].
Knowing that chemical vapour deposition (CVD) could give SWNTs with a diameter of 0.6–1.2 nm, researchers tried the same catalyst as used in CVD on arc discharge. Not all of the catalysts used appeared to result in nanotubes for both methods. But there seemed to be a correlation of diameter of SWNTs synthesised by CVD and arc discharge As a result, the diameter can be controllably lowered to a range of 0.6-1.2 nm with arc-discharge. Using a mixture of Co and Mo in high concentrations as catalyst resulted in this result. These diameters are considerably smaller than 1.2-1.4 nm16, which is the usual size gained from arcdischarge.
The torch arc aimed at the edge of the target and the soot was deposited on the substrate behind the target (see Figure ). The arc was operated at a direct current of 100 A. and shielding argon gas flowed through the torch, enhancing the arc jet formation beyond the target.
Figure 2-7: SEM images of MWNTs synthesised with (a) and without (b) the magnetic field.
At a rotation speed of 5000 rpm a yield of 60 % was found at a formation temperature of 1025 °C without the use of a catalyst. The yield increases up to 90% after purification if the rotation speed is increased and the temperature is enlarged to 1150 °C. The diameter size was not mentioned in this publication.